Robust Metal−Organic Framework Containing Benzoselenadiazole for Highly Eﬃcient Aerobic Cross-dehydrogenative Coupling Reactions under Visible Light Wen-Qiang Zhang,†,‡ Qiu-Yan Li,†,‡ Quan Zhang,§ Yingqiao Lu,† Han Lu,† Wenguang Wang,⊥ Xinsheng Zhao,∥ and Xiao-Jun Wang*,† †
Jiangsu Key Laboratory of Green Synthetic Chemistry for Functional Materials, School of Chemistry and Chemical Engineering, Jiangsu Normal University, Xuzhou 221116, P. R. China § Key Laboratory of Carbohydrate Chemistry and Biotechnology, Ministry of Education, School of Biotechnology, Jiangnan University, Wuxi 214122, P. R. China ⊥ School of Chemistry and Chemical Engineering, Shandong University, Jinan 250100, P. R. China ∥ School of Physics and Electronic Engineering, Jiangsu Normal University, Xuzhou 221116, P. R. China S Supporting Information *
incorporated noble-metal complexes, such as ruthenium(II), into UiO-67 MOFs for eﬃcient aza-Henry reactions, oxidation of sulﬁdes, and oxidative coupling of amines.13a The polypyridylruthenium complex was also introduced into UiO-67 MOFs via postsynthetic methods toward the aerobic oxidation of arylboronic acids.13b Duan et al. have utilized zinc-based MOFs consisting of triphenylamine for asymmetric α-alkylation of aldehydes with good enantioselectivity.13c Very recently, MOFs based on porphyrins and metalloporphyrins were developed as photoredox catalysts.13d,e Although large progress has been made in MOF-based photocatalysts for organic reactions, there are still some challenges to be tackled, such as the complicated synthesis of porphyrins and the possible leaching of toxic elements caused by the decomposition of noble-metal complexes. Herein, we reported a straightforward construction of benzoselenadiazole containing the MOF UiO-68Se by an approach of mixed dicarboxylate struts (H21 and H22; Figure 1), which has the robust parent UiO-68 Zr 6 O4(OH) 4(TPDC)6 framework (TPDC = terphenyl-4,4″-dicarboxylic acid)14 and exhibits a highly eﬃcient and recycalable photocatalytic activity for aerobic CDC reactions of tertiary amines and various carbon nucleophiles under visible light.
ABSTRACT: A zirconium(IV)-based UiO-topological metal−organic framework (UiO-68Se) containing benzoselenadiazole was synthesized by an approach of the mixed dicarboxylate struts, which show highly eﬃcient and recycalable photocatalytic activity for aerobic crossdehydrogenative coupling reactions between tertiary amines and various carbon nucleophiles under visiblelight irradiation.
he cross-dehydrogenative coupling (CDC) reactions from two diﬀerent C−H bonds under oxidative conditions provide a simple and atom-economic method for the construction of C−C bonds,1 because it could avoid the tedious pre- and defunctionalization of substrates. The past 10 years have witnessed huge progress in this ﬁeld.1,2 In particular, the recent development of visible-light-driven CDC reactions in the presence of photoredox catalysts via single-electron transfer (SET) has gained signiﬁcant interest because of the mild and environmentally benign characteristics.3 Various metal4 and metal-free5 photocatalysts have been employed to eﬃciently promote the cross-coupling reactions. However, most of these reactions were conducted homogeneously. There are only a few heterogeneous photocatalysts for CDC reactions.6 Metal−organic frameworks (MOFs)7 are built by the coordination self-assembly of metal ions or clusters and multidentate organic linkers, which have exhibited highly promising applications in a wide variety of areas.8 In contrast to pure inorganic materials such as metal oxide based heterogeneous photocatalysts,6c,d the hybrid and modular nature of MOFs allows a quite higher level of tailorability through ligand design,9 postsynthetic modiﬁcation,10 and postsynthetic exchange,11 thus resulting in the superior properties of MOFs. Indeed, many photoactive MOFs have recently been prepared for the degradation of organic pollutants, water splitting, and CO2 reduction toward solar energy utilization.12 On the other hand, less eﬀort has been devoted to visible-light-induced sophisticated organic transformations.13 Lin’s group ﬁrst © 2016 American Chemical Society
Figure 1. Schematic representation of the preparation for the MOF UiO-68Se. Received: November 16, 2015 Published: January 14, 2016 1005
DOI: 10.1021/acs.inorgchem.5b02626 Inorg. Chem. 2016, 55, 1005−1007
The heterogeneity of the MOF UiO-68Se was conﬁrmed by removal of the catalyst after 1 h (yield: 32%), which resulted in almost no further production of 3a after another 4 h of irradiation. This indicates that UiO-68Se acts as a purely heterogeneous catalyst with no leaching of catalytically active species into solution. The reusability of the UiO-68Se catalyst was also investigated. The same batch of UiO-68Se for the reaction of 1a and nitromethane was performed over ﬁve successive catalytic cycles (Figure S10 in the SI). The results indicate that no obvious loss of activity of the catalyst occurs even after ﬁve cycles (yield: 78%). Besides, powder XRD measurements of the recycled photocatalyst revealed maintenance of its crystalline structure and framework (Figure 2), conﬁrming the high stability of robust UiO frameworks.
The new simple ligand H21, a benzoselenadiazole-functionalized TPDC, was conveniently synthesized in high yield, as described in Scheme S1 in the Supporting Information (SI). Dimethyl-substituted TPDC H22 (Scheme S2 in the SI), owing to much better solubility, was synthesized to replace the original TPDC for preparation of the UiO-68 framework. Because of the same length of the two ligands, we utilized the mix-and-match synthetic strategy13a,15 to construct a benzoselenadiazole-doped UiO-68 MOF (UiO-68Se). Speciﬁcally, UiO-68Se was synthesized by heating the mixture of ZrCl4 and a combination of ligands H21 and H22 in N,N′-dimethylformamide using HAc as an additive at 100 °C for 2 days (for details, see the SI). Powder X-ray diﬀraction (XRD) conﬁrmed its highly crystalline nature and the fact that it is isostructural with the parent UiO-68 framework (Figure S2 in the SI). Nitrogen sorption measurement at 77 K revealed a typical type I reversible isotherm with Brunauer−Emmett−Teller surface area of up to ∼3500 m2 g−1 (Figure S9 in the SI), indicating its high porosity. Because of the presence of large open channels that will facilitate the diﬀusion of substrates and products, UiO-68Se was used as the heterogeneous photocatalyst for an aerobic CDC model reaction of N-phenyl-1,2,3,4-tetrahydroisoquinoline (1a) with nitromethane. As shown in Table 1, for a mixture of 1a and Table 1. Screening of the Reaction Conditionsa
Figure 2. Powder XRD patterns for UiO-68Se. entry
1 2 3 4 5c 6d 7e 8f
UiO-68Se, 2 mg UiO-68Se, 2 mg UiO-68Se, 4 mg UiO-68Se, 4 mg UiO-68M, 4 mg no catalyst no light no oxygen
2 4 2 4 4 4
76 89 86 100 trace trace 0 0
68 84 82 90 trace trace n.r. n.r.
It has been demonstrated that oxygen played an important role in the photoinduced aerobic CDC reactions.4,5 To understand the MOF UiO-68Se photocatalysed process clearly, electron spin resonance (ESR) measurements were conducted in which 2,2,6,6-tetramethylpiperidine (TEMP) and 5,5-dimethyl-1pyrroline-N-oxide (DMPO) were used to capture singlet oxygen 1 O2 and superoxide radical anion O2•−, respectively. As shown in Figure 3, upon irradiation of the CH3CN mixture of UiO-68Se
Reaction conditions: 1a (0.1 mmol) and CH3NO2 (1.0 mL), blue LEDs (λmax = 450 nm, 3 W). The reaction with stirring was conducted in an air atmosphere at room temperature. bYield and conversion determined by 1H NMR using methyl 3,5-dinitrobenzoate as an internal standard. n.r. = no reaction. cThe reaction in the presence of UiO-68M was irradiated for 4 h. dThe reaction without any catalyst was irradiated for 4 h. eThe reaction in the presence of UiO-68Se was stirred in the dark for 6 h. fThe reaction mixture was strictly degassed by nitrogen for 6 h and then irradiated under a nitrogen atmosphere for 4 h.
nitromethane containing a catalytic amount of UiO-68Se under irradiation of blue LEDs at ambient conditions for several hours, we observed formation of the desired cross-coupling product 3a in good-to-excellent yield (entries 1−4). As expected, increasing the amount of catalyst and irradiation time gives high conversation and yield (entry 4). The inactivity of the parent MOF UiO-68M in this reaction conﬁrmed that the benzoselenadiazole-functionalized TPDC ligand in UiO-68Se acts as a photocatalytically active center for this process (entry 5). Other control experiments demonstrated that each component of the reaction, including light, oxygen, and the MOF photocatalyst, is essential for the progress of the aerobic CDC reaction (entries 6−8).
Figure 3. ESR spectra of a solution in CH3CN of UiO-68Se without 1a (a) and with 1a (b) in the presence of DMPO under irradiation of blue LEDs for 30 s and a solution in CH3CN of UiO-68Se without 1a (c) and with 1a (d) in the presence of TEMP under irradiation of blue LEDs for 30 s.
and TEMP in air, a typically characteristic signal of 1O2 was clearly observed. However, the signal disappeared upon the addition of 1a to the mixture. By contrast, a clear characteristic signal of O2•− was detected when DMPO was used as the radical scavenger. These ﬁndings indicate that O2•− is the active intermediate species in the reaction rather than 1O2. 1006
DOI: 10.1021/acs.inorgchem.5b02626 Inorg. Chem. 2016, 55, 1005−1007
5992−5995. (d) Wan, M.; Lou, H.; Liu, L. Chem. Commun. 2015, 51, 13953−13956. (3) (a) Beatty, J. W.; Stephenson, C. R. J. Acc. Chem. Res. 2015, 48, 1474−1484. (b) Prier, C. K.; Rankic, D. A.; MacMillan, D. W. C. Chem. Rev. 2013, 113, 5322−5363. (c) Narayanam, J. M. R.; Stephenson, C. R. J. Chem. Soc. Rev. 2011, 40, 102−113. (d) Xuan, J.; Xiao, W.-J. Angew. Chem., Int. Ed. 2012, 51, 6828−6838. (e) Shi, L.; Xia, W. Chem. Soc. Rev. 2012, 41, 7687−7697. (4) (a) Wu, C.-J.; Zhong, J.-J.; Meng, Q.-Y.; Lei, T.; Gao, X.-W.; Tung, C.-H.; Wu, L.-Z. Org. Lett. 2015, 17, 884−887. (b) Zhong, J.-J.; Meng, Q.-Y.; Wang, G.-X.; Liu, Q.; Chen, B.; Feng, K.; Tung, C.-H.; Wu, L.-Z. Chem. - Eur. J. 2013, 19, 6443−6450. (c) Condie, A. G.; GonzálezGómez, J. C.; Stephenson, C. R. J. J. Am. Chem. Soc. 2010, 132, 1464− 1465. (d) Zou, Y.-Q.; Lu, L.-Q.; Fu, L.; Chang, N.-J.; Rong, J.; Chen, J.R.; Xiao, W.-J. Angew. Chem., Int. Ed. 2011, 50, 7171−7175. (5) (a) Nicewicz, D. A.; Nguyen, T. M. ACS Catal. 2014, 4, 355−360. (b) Wang, X.-Z.; Meng, Q.-Y.; Zhong, J.-J.; Gao, X.-W.; Lei, T.; Zhao, L.M.; Li, Z.-J.; Chen, B.; Tung, C.-H.; Wu, L.-Z. Chem. Commun. 2015, 51, 11256−11259. (c) Liu, Q.; Li, Y.-N.; Zhang, H.-H.; Chen, B.; Tung, C.H.; Wu, L.-Z. Chem. - Eur. J. 2012, 18, 620−627. (d) Meng, Q.-Y.; Zhong, J.-J.; Liu, Q.; Gao, X.-W.; Zhang, H.-H.; Lei, T.; Li, Z.-J.; Feng, K.; Chen, B.; Tung, C.-H.; Wu, L.-Z. J. Am. Chem. Soc. 2013, 135, 19052−19055. (6) (a) Chen, J.; Cen, J.; Xu, X.; Li, X. Catal. Sci. Technol. 2016, DOI: 10.1039/C5CY01289A. (b) Jana, A.; Mondal, J.; Borah, P.; Mondal, S.; Bhaumik, A.; Zhao, Y. Chem. Commun. 2015, 51, 10746− 10749. (c) Rueping, M.; Zoller, J.; Fabry, D. C.; Poscharny, K.; Koenigs, R. M.; Weirich, T. E.; Mayer, J. Chem. - Eur. J. 2012, 18, 3478−3481. (d) Wang, J.; Ma, J.; Li, X.; Li, Y.; Zhang, G.; Zhang, F.; Fan, X. Chem. Commun. 2014, 50, 14237−14240. (7) (a) Allendorf, M. D.; Stavila, V. CrystEngComm 2015, 17, 229−246. (b) Zhou, H.-C.; Kitagawa, S. Chem. Soc. Rev. 2014, 43, 5415−5418. (c) Zhou, H.-C.; Long, J. R.; Yaghi, O. M. Chem. Rev. 2012, 112, 673− 674. (8) (a) Chughtai, A. H.; Ahmad, N.; Younus, H. A.; Laypkov, A.; Verpoort, F. Chem. Soc. Rev. 2015, 44, 6804−6849. (b) Xia, W.; Mahmood, A.; Zou, R.; Xu, Q. Energy Environ. Sci. 2015, 8, 1837−1866. (c) Cui, Y.; Zhu, F.; Chen, B.; Qian, G. Chem. Commun. 2015, 51, 7420− 7431. (d) He, C.; Liu, D.; Lin, W. Chem. Rev. 2015, 115, 11079−11108. (9) (a) Lu, W.; Wei, Z.; Gu, Z.-Y.; Liu, T.-F.; Park, J.; Park, J.; Tian, J.; Zhang, M.; Zhang, Q.; Gentle Iii, T.; Bosch, M.; Zhou, H.-C. Chem. Soc. Rev. 2014, 43, 5561−5593. (b) Zhang, M.; Bosch, M.; Gentle Iii, T.; Zhou, H.-C. CrystEngComm 2014, 16, 4069−4083. (10) (a) Cohen, S. M. Chem. Rev. 2012, 112, 970−1000. (b) Wang, Z.; Cohen, S. M. Chem. Soc. Rev. 2009, 38, 1315−1329. (11) (a) Deria, P.; Mondloch, J. E.; Karagiaridi, O.; Bury, W.; Hupp, J. T.; Farha, O. K. Chem. Soc. Rev. 2014, 43, 5896−5912. (b) Fei, H.; Cohen, S. M. J. Am. Chem. Soc. 2015, 137, 2191−2194. (12) (a) Zhang, T.; Lin, W. Chem. Soc. Rev. 2014, 43, 5982−5993. (b) Wang, C.-C.; Li, J.-R.; Lv, X.-L.; Zhang, Y.-Q.; Guo, G. Energy Environ. Sci. 2014, 7, 2831−2867. (c) Meyer, K.; Ranocchiari, M.; van Bokhoven, J. A. Energy Environ. Sci. 2015, 8, 1923−1937. (d) Wang, S.; Wang, X. Small 2015, 11, 3097−3112. (13) (a) Wang, C.; Xie, Z.; deKrafft, K. E.; Lin, W. J. Am. Chem. Soc. 2011, 133, 13445−13454. (b) Yu, X.; Cohen, S. M. Chem. Commun. 2015, 51, 9880−9883. (c) Wu, P.; He, C.; Wang, J.; Peng, X.; Li, X.; An, Y.; Duan, C. J. Am. Chem. Soc. 2012, 134, 14991−14999. (d) Johnson, J. A.; Luo, J.; Zhang, X.; Chen, Y.-S.; Morton, M. D.; Echeverría, E.; Torres, F. E.; Zhang, J. ACS Catal. 2015, 5, 5283−5291. (e) Toyao, T.; Ueno, N.; Miyahara, K.; Matsui, Y.; Kim, T.-H.; Horiuchi, Y.; Ikeda, H.; Matsuoka, M. Chem. Commun. 2015, 51, 16103−16106. (14) Cavka, J. H.; Jakobsen, S.; Olsbye, U.; Guillou, N.; Lamberti, C.; Bordiga, S.; Lillerud, K. P. J. Am. Chem. Soc. 2008, 130, 13850−13851. (15) Siu, P. W.; Brown, Z. J.; Farha, O. K.; Hupp, J. T.; Scheidt, K. A. Chem. Commun. 2013, 49, 10920−10922.
We proposed a plausible reaction mechanism based on the above results (Scheme S3 in the SI). Upon excitation of UiO68Se (PS), SET from 1a to PS* occurs with generation of the radical cation 1a•+ and the radical anion PS•−, which transfer an electron to O2 with the formation of O2•− and the simultaneous regeneration of the ground-state PS. Meanwhile, O2•− abstracts a proton from 1a•+, generating a hydroperoxide free radical and intermediate 1a•. The latter lose one electron to aﬀord the imine cation, followed by nucleophile addition to give the product 3a. With a well understanding of the reaction mechanism, we further extended the scope of this aerobic CDC reaction photocatalyzed by the MOF UiO-68Se shown in Table S1 (SI). It can be observed that various substituted tetrahydroisoquinoline derivatives can undergo aerobic CDC reactions with diﬀerent nitroalkanes catalyzed by UiO-68Se under visible light, giving the coupling products in good-to-excellent yields. Moreover, the MOF-photocatalyzed CDC reaction can also be expanded to the direct construction of C−C bonds between N-aryltetrahydroisoquinolines with dialkyl malonates and ketones, with satisfactory yields (Table S2 in the SI). In summary, we designed and synthesized a simple benzoselenadiazole-functionalized TPDC ligand. Subsequently, a noble-metal-free Zr-MOF with a UiO-68 framework was constructed by the straightforward reaction of ZrCl4 with the mixed dicarboxylate struts. The robust MOF can act as a highly eﬃcient and heterogeneous photoredox catalyst for aerobic CDC reactions between tertiary amines with various carbon nucleophiles under visible light. It is envisioned that the MOF can act as an ideal platform, allowing for the incorporation of more photoredox catalysts.
S Supporting Information *
The Supporting Information is available free of charge on the ACS Publications website at DOI: 10.1021/acs.inorgchem.5b02626. Experimental details, thermogravimetric analysis and nitrogen sorption of UiO-68Se, and other details (PDF)
*E-mail: [email protected]
. Author Contributions ‡
These authors contributed equally.
The authors declare no competing ﬁnancial interest.
ACKNOWLEDGMENTS We are grateful for ﬁnancial support from NSFC (Grants 21302072, 51403081, and 21376113), NSF of Jiangsu Province (Grants BK20130226 and BK20140137), and PAPD of Jiangsu Higher Education Institutions.
(1) (a) Girard, S. A.; Knauber, T.; Li, C.-J. Angew. Chem., Int. Ed. 2014, 53, 74−100. (b) Yeung, C. S.; Dong, V. M. Chem. Rev. 2011, 111, 1215− 1292. (c) Scheuermann, C. J. Chem. - Asian J. 2010, 5, 436−451. (d) Li, C.-J. Acc. Chem. Res. 2009, 42, 335−344. (2) (a) Murahashi, S.-I.; Komiya, N.; Terai, H.; Nakae, T. J. Am. Chem. Soc. 2003, 125, 15312−15313. (b) Li, Z. P.; Li, C. J. J. Am. Chem. Soc. 2005, 127, 3672−3673. (c) Meng, Q.-Y.; Liu, Q.; Zhong, J.-J.; Zhang, H.-H.; Li, Z.-J.; Chen, B.; Tung, C.-H.; Wu, L.-Z. Org. Lett. 2012, 14, 1007
DOI: 10.1021/acs.inorgchem.5b02626 Inorg. Chem. 2016, 55, 1005−1007